Synthesis, structure and magnetic properties of honeycomb-layered Li3Co2SbO6 with new data on its sodium precursor, Na3Co2SbO6
Stratan, Mikhail I.; Shukaev, Igor L.; Vasilchikova, Tatyana M.; Vasiliev, Alexander N.; Korshunov, Artem N.; Kurbakov, Alexander I.; Nalbandyan, Vladimir B.; Zvereva, Elena A.; New Journal of Chemistry 43 (2019) 13545–; doi:10.1039/C9NJ03627J

data_7058714
_publ_section_title
;
 Synthesis, structure and magnetic properties of honeycomb-layered
 Li3Co2SbO6 with new data on its sodium precursor, Na3Co2SbO6
;
_journal_issue                   34
_journal_name_full               'New Journal of Chemistry'
_journal_page_first              13545
_journal_paper_doi               10.1039/C9NJ03627J
_journal_volume                  43
_journal_year                    2019
_chemical_formula_moiety         'Co2 Li3 O6 Sb'
_chemical_formula_sum            'Co2 Li3 O6 Sb'
_chemical_formula_weight         356.43
_chemical_name_common            'lithium cobalt antimonate'
_chemical_name_systematic        'lithium cobalt(+2) antimony oxide'
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_date             2016-01-10T22:06
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
;
2018-12-07 deposited with the CCDC.    2019-08-02 downloaded from the CCDC.
;
_cell_angle_alpha                90.0
_cell_angle_beta                 110.0493(22)
_cell_angle_gamma                90.0
_cell_formula_units_Z            2
_cell_length_a                   5.24111(16)
_cell_length_b                   9.03910(23)
_cell_length_c                   5.18179(12)
_cell_measurement_temperature    298
_cell_volume                     230.610(11)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  Rigaku
_diffrn_radiation_polarisn_ratio 0.707
_diffrn_radiation_probe          x-ray
_exptl_absorpt_correction_T_max  1.00126
_exptl_absorpt_correction_T_min  0.75730
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 2
 Surface roughness abs. correction (Pitschke, et al.)
Terms =     0.89940E-01    0.70358E-01
Correction is refined.
;
_exptl_crystal_density_diffrn    5.133
_exptl_crystal_preparation       'Magnetic properties'
_pd_block_id
2016-01-10T22:06|LI3CO2SBO6_ILS_VAR_8|ils|rigaku
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  reddish-brown
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        99.98
_pd_meas_2theta_range_min        6.02
_pd_meas_number_of_points        4699
_pd_meas_scan_method             cont
_pd_phase_name                   Li3Co2SbO6
_pd_proc_2theta_range_inc        0.02
_pd_proc_2theta_range_max        99.98
_pd_proc_2theta_range_min        6.02
_pd_proc_info_datetime           2016-01-10T22:06:21
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 18 terms.
 Shifted Chebyshev function of 1st kind
      1:    512.353     2:   -359.393     3:    148.202     4:   -51.3893    
      5:    44.0575     6:   -60.6529     7:    57.4487     8:   -34.6864    
      9:    11.6516    10:   -3.68274    11:  -0.319548    12:    3.20568    
     13:   -2.47042    14:  -0.793810    15:    10.0951    16:   -10.7257    
     17:   -1.46775    18:    4.70860    
;
_pd_proc_ls_peak_cutoff          0.00040
_pd_proc_ls_pref_orient_corr
;   March-Dollase
 AXIS  1 Ratio=     0.993 Frac     1.000  h= 0.000  k= 0.000  l= 1.000
 AXIS  2 Ratio=     1.000 Frac     0.000  h= 0.000  k= 1.000  l= 0.000
 Prefered orientation correction range: Min=   0.99008, Max=   1.02014
;
_pd_proc_ls_profile_function
;
 CW Profile function number 3 with  19 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 #1(GU)   =  665.942 #2(GV)   = -185.705 #3(GW)   =   17.836
 #4(GP)   =   21.129 #5(LX)   =    8.300 #6(LY)   =   10.762
 #7(S/L)  =   0.0068 #8(H/L)  =   0.0068
 #9(trns) =    -5.05 #10(shft)=   3.4998
 #11(stec)=    36.97 #12(ptec)=    -1.38 #13(sfec)=    80.17
 #14(L11) =   -0.682 #15(L22) =    0.015 #16(L33) =   -1.801
 #17(L12) =   -0.055 #18(L13) =   -0.895 #19(L23) =    0.299
 Peak tails are ignored  where the intensity is below 0.0004 times the peak
   Stacking fault sublattice vectors:
             0.0   0.0   1.0;   2.0   1.0   0.0;   0.0   3.0   0.0
;
_pd_proc_ls_prof_R_factor        0.0558
_pd_proc_ls_prof_wR_expected     0.0337
_pd_proc_ls_prof_wR_factor       0.0753
_pd_proc_number_of_points        4699
_pd_spec_mount_mode              reflection
_pd_spec_shape                   flat_sheet
_refine_ls_goodness_of_fit_all   2.25
_refine_ls_matrix_type           full
_refine_ls_number_parameters     56
_refine_ls_number_restraints     12
_refine_ls_R_Fsqd_factor         0.03259
_refine_ls_shift/su_max          0.07
_refine_ls_shift/su_mean         0.01
_reflns_d_resolution_high        1.009
_reflns_d_resolution_low         4.868
_reflns_limit_h_max              5
_reflns_limit_h_min              0
_reflns_limit_k_max              10
_reflns_limit_k_min              0
_reflns_limit_l_max              5
_reflns_limit_l_min              -5
_reflns_number_total             256
_cod_data_source_file            c9nj03627j1.cif
_cod_data_source_block           LI3CO2SBO6_ILS_VAR_8_publ
_cod_depositor_comments          'Adding full bibliography for 7058714.cif.'
_cod_original_sg_symbol_Hall     '-c 2y'
_cod_database_code               7058714
_publcif_datablock.id            {96dad6ff-9cd3-4f91-8717-be00ccc008e2}
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000